Presentation on theme: "Presentation downloadable from www.tececo.com TecEco Cements – Making Concrete Foolproof There are two fundamental factors affecting durability: transport."— Presentation transcript:
Presentation downloadable from TecEco Cements – Making Concrete Foolproof There are two fundamental factors affecting durability: transport and reactivity of reactants Bad work is costly, looks lousy and usually compromises long term durability.
Presentation downloadable from What Influences Durability? Concretes are said to be less durable when they are physically or chemically compromised. Physical factors can result in chemical reactions reducing durability –E.g Cracking due to shrinkage can allow reactive gases and liquids to enter the concrete Chemical factors can result in physical outcomes reducing durability –E.g Alkali silica reaction opening up cracks allowing other agents such as sulfate and chloride in seawater to enter. This presentation will describe benchmark improvements in durability as a result of using the new TecEco magnesian cement technologies
Presentation downloadable from Many Engineering Issues are Actually Mineralogical Issues Problems with Portland cement concretes are usually resolved by the band aid engineering fixes. e.g. –Use of calcium nitrite, silanes, cathodic protection or stainless steel to prevent corrosion. –Use of coatings to prevent carbonation. –Crack control joins to mitigate the affects of shrinkage cracking. –Plasticisers to improve workability. Portlandite and water are the weakness of concrete –TecEco remove Portlandite it and replacing it with magnesia which hydrates to Brucite. –The hydration of magnesia consumes significant water
Presentation downloadable from TecEco Binder Theory Portlandite (Ca(OH) 2 ) is too soluble, mobile and reactive. –It carbonates, reacts with Cl - and SO 4 - and being soluble can act as an electrolyte. TecEco generally (but not always) remove Portlandite using the pozzolanic reaction and TecEco add reactive magnesia –which hydrates, consuming significant water and concentrating alkalis forming B rucite which is another alkali, but much less soluble, mobile or reactive than Portlandite. In Eco-cements brucite carbonates
Presentation downloadable from TecEco Binder Systems Hydration of the various components of Portland cement for strength. SUSTAINABILITY DURABILITYSTRENGTH TECECO CEMENTS Reaction of alkali with pozzolans (e.g. lime with fly ash.) for sustainability, durability and strength. Hydration of magnesia => brucite fo strength, workability, dimensional stability and durability. In Eco-cements carbonation of brucite => nesquehonite, lansfordite and an amorphous phase for sustainability. PORTLAND POZZOLAN REACTIVE MAGNESIA TecEco concretes are a system of blending reactive magnesia, Portland cement and usually a pozzolan with other materials and are a key factor for sustainability.
Presentation downloadable from Why Add Reactive Magnesia? To maintain the long term stability of CSH. –Maintains alkalinity preventing the reduction in Ca/Si ratio. To remove water. –Reactive magnesia consumes water as it hydrates to possibly hydrated forms of Brucite. To raise the early Ph. –Increasing non hydraulic strength giving reactions To reduce shrinkage. –The consequences of putting brucite through the matrix of a concrete in the first place need to be considered. To make concretes more durable Because significant quantities of carbonates are produced in porous substrates which are affective binders. Reactive MgO is a new tool to be understood with profound affects on most properties
Presentation downloadable from TecEco Formulations Tec-cements (5-15% MgO, 85-95% OPC) –contain more Portland cement than reactive magnesia. Reactive magnesia hydrates in the same rate order as Portland cement forming Brucite which uses up water reducing the voids:paste ratio, increasing density and possibly raising the short term pH. –Reactions with pozzolans are more affective. After all the Portlandite has been consumed Brucite controls the long term pH which is lower and due to its low solubility, mobility and reactivity results in greater durability. –Other benefits include improvements in density, strength and rheology, reduced permeability and shrinkage and the use of a wider range of aggregates many of which are potentially wastes without reaction problems. Eco-cements (15-95% MgO, 85-5% OPC) –contain more reactive magnesia than in tec-cements. Brucite in porous materials carbonates forming stronger fibrous mineral carbonates and therefore presenting huge opportunities for waste utilisation and sequestration. Enviro-cements (5-15% MgO, 85-95% OPC) –contain similar ratios of MgO and OPC to eco-cements but in non porous concretes brucite does not carbonate readily. –Higher proportions of magnesia are most suited to toxic and hazardous waste immobilisation and when durability is required. Strength is not developed quickly nor to the same extent.
Presentation downloadable from Tec-Cement Reactions MgO + H 2 O => Mg(OH) 2.nH 2 O - water consumption resulting in greater density and higher alkalinity. Higher alkalinity => more reactions involving silica & alumina. Mg(OH) 2.nH 2 O => Mg(OH) 2 + H 2 O – slow release water for more complete hydration of PC MgO + Al + H 2 O => 3MgO.Al.6H 2 O ??? – equivalent to flash set?? MgO + SO 4 -- => various Mg oxy sulfates ?? – yes but more likely ettringite reaction consumes SO 4 -- first. MgO + SiO 2 => MSH ?? Yes but high alkalinity required. Strength?? We think the reactions are relatively independent of PC reactions
Presentation downloadable from The Form of MgO Matters - Lattice Energy Destroys a Myth Magnesia, provided it is reactive rather than dead burned (or high density, crystalline periclase type), can be beneficially added to cements in excess of the amount of 5 mass% generally considered as the maximum allowable by standards prevalent in concrete dogma. –Reactive magnesia is essentially amorphous magnesia with low lattice energy. –It is produced at low temperatures and finely ground, and –will completely hydrate in the same time order as the minerals contained in most hydraulic cements. Dead burned magnesia and lime have high lattice energies –Crystalline magnesium oxide or periclase has a calculated lattice energy of 3795 Kj mol-1 which must be overcome for it to go into solution or for reaction to occur. –Dead burned magnesia is much less expansive than dead burned lime in a hydraulic binder (Ramachandran V. S., Concrete Science, Heydon & Son Ltd. 1981, p )
Presentation downloadable from Crack Collage TecEco technology can reduce if not solve problems of cracking: –Related to (shrinkage) through open system loss of water. –As a result of volume change caused by delayed reactions –As a result of corrosion. –Related to autogenous shrinkage Thermal Plastic Shrinkage Drying Shrinkage Corrosion Related Freeze Thaw D Cracks Structural Settlement Shrinkage Photos from PCA and US Dept. Ag Websites Autogenous or self-desiccation shrinkage (usually related to stoichiometric or chemical shrinkage) Alkali aggregate Reaction Evaporative Crazing Shrinkage
Presentation downloadable from Causes of Cracking in Concrete Cracking commonly occurs when the induced stress exceeds the maximum tensile stress capacity of concrete and can be caused by many factors including restraint, extrinsic loads, lack of support, poor design, volume changes over time, temperature dependent volume change, corrosion or delayed reactions. Causes of induced stresses include: –Restrained thermal, plastic, drying and stoichiometric shrinkage, corrosion and delayed reaction strains. –Slab curling. –Loading on concrete structures. Cracking is undesirable for many reasons –Visible cracking is unsightly –Cracking compromises durability because it allows entry of gases and ions that react with Portlandite. –Cracking can compromise structural integrity, particularly if it accelerates corrosion.
Presentation downloadable from Graphic Illustration of Cracking After Tony Thomas (Boral Ltd.) (Thomas 2005) Autogenous shrinkage has been used to refer to hydration shrinkage and is thus stoichiometric
Presentation downloadable from Cracking due to Loss of Water Drying Shrinkage Plastic Shrinkage Picture from: Evaporative Crazing Shrinkage Settlement Shrinkage We may not be able to prevent too much water being added to concrete by fools. TecEco approach the problem in a different way by providing for the internal removal/storage of water that can provide for more complete hydration of PC. Brucite gains weight in excess of the theoretical increase due to MgO conversion to Mg(OH)2 in samples cured at 98% RH. Dr Luc Vandepierre, Cambridge University, 20 September, Bucket of Water Fool
Presentation downloadable from Solving Cracking due Shrinkage from Loss of Water In the system water plus Portland cement powder plus aggregates shrinkage is in the order of.05 – 1.5 %. There are two root causes of Portland cements shrinking over time. –Stoichiometric (chemical) shrinkage and –Shrinkage through loss of water. The solution is to: –Add minerals that compensate by stoichiometrically expanding and/or to –Use less water, internally hold water or prevent water loss. TecEco tec-cements internally hold water and prevent water loss. MgO (s) + H 2 O (l) Mg(OH) 2.nH 2 O (s)
Presentation downloadable from When magnesia hydrates it consumes 18 litres of water per mole of magnesia probably more depending on the value of n in the reaction below: MgO (s) + H 2 O (l) Mg(OH) 2. nH2O (s) The dimensional change in the system MgO + PC depends on: –The ratio of MgO to PC –Whether water required for hydration of PC and MgO is coming from stoichiometric mix water (i.e the amount calculated as required), excess water (bleed or evaporative) or from outside the system. –In practice tec-cement systems are more closed and thus dimensional change is more a function of the ratio of MgO to PC As a result of preventing the loss of water by closing the system together with expansive stoichiometry of MgO reactions (see below). MgO (s) + H 2 O (l) Mg(OH) 2. nH2O (s) molar mass (at least!) liquid 24.3 molar volumes (at least!) It is possible to significantly reduce if not prevent (drying, plastic, evaporative and some settlement) shrinkage as a result of water losses from the system. The molar volume (L.mol-1)is equal to the molar mass (g.mol-1) divided by the density (g.L-1). Preventing Shrinkage through Loss of Water
Presentation downloadable from Portland cements stoichiometrically require around % water for hydration yet we add approximately 45 to 60% at cement batching plants to fluidise the mix sufficiently for placement. If it were not for the enormous consumption of water by tri calcium aluminate as it hydrates forming ettringite in the presence of gypsum, concrete would remain as a weak mush and probably never set. –26 moles of water are consumed per mole of tri calcium aluminate to from a mole of solid ettringite. When the ettringite later reacts with remaining tri calcium aluminate to form monosulfoaluminate hydrate a further 4 moles of water are consumed. The addition of reactive MgO achieves water removal internally in a closed system in a similar way. Preventing Shrinkage through Loss of Water MgO (s) + H 2 O (l) Mg(OH) 2.nH 2 O (s)
Presentation downloadable from Stop Press – Confirmation of Brucite Hydrates UK Student 17/10/05 to John Harrison Brucite indeed gains more weight when cured at 98% RH forming probably a Mg(OH) 2.nH 2 O phase. Further research is under way to establish the stability and nature of this phase (what is n number and whether it desiccates). So far, thermogravimetric analysis showed that the weight loss of Mg(OH) 2.nH 2 O --> MgO is between 39% and 42%, significantly more than the expected 30.8% (Mg(OH) 2 --> MgO).
Presentation downloadable from Other Benefits of Preventing Shrinkage through Loss of Water Internal water consumption also results in: –Greater strength More complete hydration of PC. Reduced in situ voids:paste ratio –Greater density Increased durability Higher short term alkalinity More effective pozzolanic reactions. More complete hydration of PC. –Small substitutions of PC by MgO result in water being trapped inside concrete as Brucite and Brucite hydrates which can later self dessicate delivering water to hydration reactions of calcium silicates (Preventing so called autogenous shrinkage).
Presentation downloadable from Bleeding is a Bad Thing Bleeding is caused by: –Lack of fines –Too much water Bleeding can be fixed by: –Reducing water or adding fines –Air entrainment or grading adjustments Bleeding causes: –Reduced pumpability –Loss of cement near the surface of concretes –Delays in finishing –Poor bond between layers of concrete –Interconnected pore structures that allow aggressive agents to enter later –Slump and plastic cracking due to loss of volume from the system –Loss of alkali that should remain in the system for better pozzolanic reactions –Loss of pollutants such as heavy metals if wastes are being incorporated. Concrete is better as a closed system Better to keep concretes as closed systems
Presentation downloadable from Open/Closed Systems - The Wet Sand Analogy In the particulate state wet beach sand is held together by the surface tension of water (a ramification of hydrogen bonding) A beach sand system emulates a closed system because water lost through evaporation or bleeding is constantly replaced by waves. No plastic or drying shrink cracking is observable in wet beach sands. To prevent plastic and drying shrink cracking in concrete the system must also be closed preventing loss of water through evaporation. To do this surface coatings such as aliphatic alcohols are used. The TecEco method is to internally hold water in brucite and its hydrates that would otherwise bleed or evaporate. Concrete can be made totally shrinkproof (foolproof) –Adding reactive magnesia to consume and store water as it hydrates. –Applying surface coatings e.g. aliphatic alcohol (e.g. ethelyene glycol). As a result joints are usually only necessary for structural reasons. Wet sand or wet concrete? Wet concrete still in the particulate stage has much in common with wet sand
Presentation downloadable from Dimensionally Control Over Concretes During Curing? Portland cement concretes shrink around.05%. Over the long term much more (>.1%). –Mainly due to plastic and drying shrinkage through loss of water The use of some wastes as aggregates also cause shrinkage e.g. wood waste in masonry units, thin panels etc.
Presentation downloadable from When magnesia hydrates it expands: MgO (s) + H 2 O (l) Mg(OH) 2. nH 2 O (s) >58.3 molar mass liquid >24.3 molar volumes Consuming significant water preventing plastic and drying shrinkage Solidus contraction/expansion depends on –The ratio of MgO to PC –Whether the water is coming from stoichiometric mix water, bleed water or from outside the system. TecEco cements are usually more closed (i.e they do not bleed) The molar volume (L.mol-1)is equal to the molar mass (g.mol-1) divided by the density (g.L-1). Volume Changes on Hydration
Presentation downloadable from Dimensional Control in Tec-Cement Concretes By adding MgO volume changes are minimised to close to neutral. –So far we have observed significantly less shrinkage in TecEco tec - cement concretes with about (8-10% substitution OPC) with or without fly ash. –At some ratio, thought to be around % reactive magnesia and 90 – 95% OPC volume changes cancel each other out. –The water lost by concrete as it shrinks is used by the reactive magnesia as it hydrates eliminating shrinkage. Note that brucite is > mass% water and it makes sense to make binders out of water! More research is required to accurately establish volume relationships.
Presentation downloadable from Balancing Time Dependent Dimensional Change
Presentation downloadable from Greater Tensile Strength also Reduces Cracking MgO Changes Surface Charge as the Ph Rises. This could be the reason for the greater tensile strength displayed during the early plastic phase of tec-cement concretes. The affect of additives is not yet known Mutual Repulsion => Ph 12 ? Cement MgO Sand MgO Mutual Repulsion Mutual Attraction
Presentation downloadable from Reducing Cracking as a Result of Volume Change caused by Delayed Reactions Photo Courtesy Ahmad Shayan ARRB An Alkali Aggregate Reaction Cracked Bridge Element
Presentation downloadable from Types of Delayed Reactions There are several types of delayed reactions that cause volume changes (generally expansion) and cracking. –Alkali silica reactions –Alkali carbonate reactions –Delayed ettringite formation –Delayed thaumasite formation –Delayed hydration or dead burned lime or periclase. Delayed reactions cause dimensional distress, cracking and possibly even failure.
Presentation downloadable from Reducing Delayed Reactions Delayed reactions do not appear to occur to the same extent in TecEco cements. –A lower long term pH results in reduced reactivity after the plastic stage. –Potentially reactive ions are trapped in the structure of brucite. –Ordinary Portland cement concretes can take years to dry out however the reactive magnesia in Tec- cement concretes consumes unbound water from the pores inside concrete. –Magnesia dries concrete out from the inside. Reactions do not occur without water.
Presentation downloadable from Reduced Corrosion Related Cracking Steel remains protected with a passive oxide coating of Fe 3 O 4 above pH 8.9. A pH of over 8.9 is maintained by the equilibrium Mg(OH) 2 Mg OH - for much longer than the pH maintained by Ca(OH) 2 because: –Brucite does not react as readily as Portlandite resulting in reduced carbonation rates and reactions with salts. Concrete with brucite in it is denser and carbonation is expansive, sealing the surface preventing further access by moisture, CO 2 and salts. Rusting Causes Dimensional Distress
Presentation downloadable from Brucite is less soluble and traps salts as it forms resulting in less ionic transport to complete a circuit for electrolysis and less corrosion. Free chlorides and sulfates originally in cement and aggregates are bound by magnesium –Magnesium oxychlorides or oxysulfates are formed. ( Compatible phases in hydraulic binders that are stable provided the concrete is dense and water kept out.) As a result of the above the rusting of reinforcement does not proceed to the same extent. Cracking or spalling due to rust does not occur Reduced Corrosion Related Cracking
Presentation downloadable from Reducing Cracking Related to Autogenous Shrinkage Autogenous shrinkage tends to occur in high performance concretes in which dense microstructures develop quickly preventing the entry of additonal water required to complete hydration. –First defined by Lynam in 1934 (Lynam CG. Growth and movement in portland cement concrete.London: Oxford University Press; p ) The autogenous deformation of concrete is defined as the unrestrained, bulk deformation that occurs when concrete is kept sealed and at a constant temperature.
Presentation downloadable from Reducing Cracking Related to Autogenous Shrinkage Main cause is stoichiometric or chemical shrinkage as observed by Le Chatelier. –whereby the reaction products formed during the hydration of cement occupy less space than the corresponding reactants. A dense cement paste hydrating under sealed conditions will therefore self-desiccate creating empty pores within developing structure. If external water is not available to fill these empty pores, considerable shrinkage can result. Le Chatelier H. Sur les changements de volume qui accompagnent Ie durcissement des ciments. Bulletin de la Societe d'Encouragement pour I'Industrie Nationale 1900:54-7.
Presentation downloadable from Reducing Cracking Related to Autogenous Shrinkage Autogenous shrinkage does not occur in high strength tec-cement concretes because: –The brucite hydrates that form desiccate back to brucite delivering water in situ for more complete hydration of Portland cement. Mg(OH) 2.nH 2 O (s) MgO (s) + H 2 O (l) As brucite is a relatively weak mineral is compressed and densifies the microstructure. –The stoichiometric shrinkage of Portland cement (first observed by Le Chatelier) is compensated for by the stoichiometric expansion of magnesium oxide on hydration. MgO (s) + H 2 O (l) Mg(OH) 2. nH 2 O (s) molar mass (at least!) liquid 24.3 molar volumes (at least 116% expansion, probably more initially before desiccation as above!)
Presentation downloadable from Easier to Finish Concretes Easier to pump and finish Concretes are likely to have less water added to them resulting in less cracking
Presentation downloadable from Non Newtonian Rheology The strongly positively charged small Mg++ atoms attract water (which is polar) in deep layers introduce a shear thinning property affecting the rheological properties and making concretes less sticky with added pozzolan It is not known how deep these layers get Etc. Ca++ = 114, Mg++ = 86 picometres
Presentation downloadable from Bingham Plastic Rheology TecEco concretes and mortars are: –Very homogenous and do not segregate easily. They exhibit good adhesion and have a shear thinning property. –Exhibit Bingham plastic qualities and react well to energy input. –Have good workability. TecEco concretes with the same water/binder ratio have a lower slump but greater plasticity and workability. TecEco tec-cements are potentially suitable for mortars, renders, patch cements, colour coatings, pumpable and self compacting concretes. A range of pumpable composites with Bingham plastic properties will be required in the future as buildings will be printed.
Presentation downloadable from Improved Durability Materials that last longer need replacing less often saving on energy and resources. Reasons for Improved Durability: –Greater Density = Lower Permeability Physical Weaknesses => Chemical Attack –Removal of Portlandite with the Pozzolanic Reaction. Removal or reactive components –Substitution by Brucite => Long Term pH control Reducing corrosion
Presentation downloadable from Reduced Permeability As bleed water exits ordinary Portland cement concretes it creates an interconnected pore structure that remains in concrete allowing the entry of aggressive agents such as SO 4 --, Cl - and CO 2 TecEco tec - cement concretes are a closed system. They do not bleed as excess water is consumed by the hydration of magnesia. –As a result TecEco tec - cement concretes dry from within, are denser and less permeable and therefore stronger more durable and less permeable. Cement powder is not lost near the surfaces. Tec-cements have a higher salt resistance and less corrosion of steel etc.
Presentation downloadable from Concretes have a high percentage (around 18% – 22%) of voids. On hydration magnesia expands >=116.9 % filling voids and surrounding hydrating cement grains => denser concrete. On carbonation to nesquehonite brucite expands 307% sealing the surface. Lower voids:paste ratios than water:binder ratios result in little or no bleed water, lower permeability and greater density. Greater Density – Lower Permeability
Presentation downloadable from Densification During the Plastic Phase Water is required to plasticise concrete for placement, however once placed, the less water over the amount required for hydration the better. Magnesia consumes water as it hydrates producing solid material. Less water results in increased density and concentration of alkalis - less shrinkage and cracking and improved strength and durability.
Presentation downloadable from Brucite has always played a protective role during salt attack. Putting it in the matrix of concretes in the first place makes sense. Brucite does not react with salts because it is a least 5 orders of magnitude less soluble, mobile or reactive. –Ksp brucite = 1.8 X –Ksp Portlandite = 5.5 X TecEco cements are more acid resistant than Portland cement –This is because of the relatively high acid resistance (?) of Lansfordite and nesquehonite compared to calcite or aragonite Durability - Reduced Salt & Acid Attack
Presentation downloadable from Substitution by Brucite => Long Term pH control TecEco add reactive magnesia which hydrates forming brucite which is another alkali, but much less soluble, mobile or reactive than Portlandite. Brucite provides long term pH control.
Presentation downloadable from Reduced Steel Corrosion Steel remains protected with a passive oxide coating of Fe 3 O 4 above pH 8.9. A pH of over 8.9 is maintained by the equilibrium Mg(OH) 2 Mg OH - for much longer than the pH maintained by Ca(OH) 2 because: –Brucite does not react as readily as Portlandite resulting in reduced carbonation rates and reactions with salts. Concrete with brucite in it is denser and carbonation is expansive, sealing the surface preventing further access by moisture, CO 2 and salts. Brucite is less soluble and traps salts as it forms resulting in less ionic transport to complete a circuit for electrolysis and less corrosion. Free chlorides and sulfates originally in cement and aggregates are bound by magnesium –Magnesium oxychlorides or oxysulfates are formed. ( Compatible phases in hydraulic binders that are stable provided the concrete is dense and water kept out.)
Presentation downloadable from Corrosion Reduced by a Lower More Stable Long Term pH Eh-pH or Pourbaix Diagram The stability fields of hematite, magnetite and siderite in aqueous solution; total dissolved carbonate = M. In TecEco cements the long term pH is governed by the low solubility and carbonation rate of brucite and is much lower at around , allowing a wider range of aggregates to be used, reducing problems such as AAR and etching. The pH is still high enough to keep Fe 3 O 4 stable in reducing conditions. Steel corrodes below 8.9 Equilibrium pH of Brucite and of lime
Presentation downloadable from Less Freeze - Thaw Problems Denser concretes do not let water in. Brucite will to a certain extent take up internal stresses When magnesia hydrates it expands into the pores left around hydrating cement grains: MgO (s) + H 2 O (l) Mg(OH) 2 (s) molar mass molar volumes molar volumes At least 38% air voids are created in space that was occupied by magnesia and water! Air entrainment can also be used as in conventional concretes TecEco concretes are not attacked by the salts used on roads
Presentation downloadable from Rosendale Concretes - Partial Proof Rosendale cements contained 14 – 30% MgO A major structure built with Rosendale cements commenced in 1846 was Fort Jefferson near key west in Florida. Rosendale cements were recognized for their exceptional durability, even under severe exposure. At Fort Jefferson much of the 150 year-old Rosendale cement mortar remains in excellent condition, in spite of the severe ocean exposure and over 100 years of neglect. Fort Jefferson is nearly a half mile in circumference and has a total lack of expansion joints, yet shows no signs of cracking or stress. The first phase of a major restoration is currently in progress. More information from
Presentation downloadable from Strength Faster & greater strength development even with added pozzolans Water removal by magnesia as it hydrates in tec-cements results in a higher short term pH and therefore more affective pozzolanic reactions. Brucite hydrate fills pore spaces taking up mix and bleed water as it hydrates reducing voids and shrinkage (brucite hydrate is > mass% water!). Greater density (lower voids:paste ratio) and lower permeability results in greater strength. Possible formation of Mg Al hydrates. Strength from self compaction Problems with Portland Cement Fixed
Presentation downloadable from Durability and Performance Permeability and Density Sulphate and chloride resistance Carbonation Corrosion of steel and other reinforcing TecEco tec - cements are Denser and much less permeable Due mainly to the removal of water by magnesia and associated volume increases Protected by brucite Which is 5 times less reactive than Portlandite Not attacked by salts, Do not carbonate readily Protective of steel reinforcing which does not corrode due to maintenance of long term pH. Problems with Portland Cement Fixed (1)
Presentation downloadable from Durability and Performance Ideal lower long term pH Delayed reactions (eg alkali aggregate and delayed ettringite) As Portlandite is removed The pH becomes governed by the pH of CSH and Brucite and Is much lower at around Stabilising many heavy metals and Allowing a wider range of aggregates to be used without AAR problems. Reactions such as carbonation are slower and The pH remains high enough to keep Fe 3 O 4 stable for much longer. Internal delayed reactions are prevented Dry from the inside out and Have a lower long term pH Problems with Portland Cement Fixed (2)
Presentation downloadable from Shrinkage Cracking, crack control Net shrinkage is reduced due to: Stoichiometric expansion of magnesium minerals, and Reduced water loss. Rheology Workability, time for and method of placing and finishing The Mg++ ion adds a shear thinning making TecEco cements very workable. Hydration of magnesia rapidly adds early strength for finishing. Problems with Portland Cement Fixed (3)
Presentation downloadable from Improved Properties TecEco cements Can have insulating properties High thermal mass and Low embodied energy. Many formulations can be reprocessed and reused. Brucite bonds well and reduces efflorescence. Properties (contd.) Fire Retardation Brucite, hydrated magnesium carbonates are fire retardants TecEco cement products put out fires by releasing CO 2 or water at relatively low temperatures. Cost No new plant and equipment are required. With economies of scale TecEco cements should be cheaper Problems with Portland Cement Fixed (4)
Presentation downloadable from Sustainability issues Emissions and embodied energies Tec, eco and enviro-cements Less binder is required for the same strength Use a high proportion of recycled materials Immobilise toxic and hazardous wastes Can use a wider range of aggregates reducing transport emissions and Have superior durability. Tec-cements Use less cement for the same strength Eco-cements reabsorb chemically released CO 2. Problems with Portland Cement Fixed (5)